# Homework 7

```UNIVERSITY OF CALIFORNIA
College of Engineering
Department of Electrical Engineering and Computer Sciences
EECS 130
Spring 2006
Professor Chenming Hu
HOMEWORK SET NO. 7
Due: Friday, 10th March, 2006
Problem 1:
If we decrease the substrate doping concentration, how will the following
correct square.) Write down any relevant equation and explain briefly how you
obtain the answer (a few words or one sentence). Assume the gate material is
N+-poly and the body is P-type.
A
B
C
D
E
Parameters
Accumulation Region Capacitance
Flat-band Voltage, Vfb
Depletion Region Capacitance
Threshold Voltage, Vt
Inversion Region Capacitance
Increase
Decrease
Unchanged
Problem 2:
The oxide thickness (Tox) and the doping concentration (Na or Nd) of the silicon substrate
can be determined using the high-frequency C-V data shown below for an MOS structure.
1.0
0.8
0.6
C/C0
High frequency
0.4
0.2
-12
-10
-8
-6
-4
-2
0
2
4
(a) Identify the regions of accumulation, depletion and inversion in the substrate
corresponding to this C-V curve. What is the doping type of the semiconductor?
(b) If the maximum capacitance of the structure C0 (which is equal to CoxArea) is
82 pF and the gate area is 4.7510-3 cm2, what is the value of Tox?
(c) Determine the concentration in the silicon substrate. Assume a uniform doping
concentration.
Problem 3:
Consider the C-V curve of a MOS capacitor in the figure (the solid line). The
capacitor area is 6400 m2. C0 = 45 pF and C1 = 5.6 pF.
Cox
C1
V
Vg
If, due to the oxide fixed charge, the C-V curve shifted from the solid line to the
dashed line with V = 0.05V, what is the charge polarity and the area density
(C/cm2) of the oxide fixed charge?
Problem 4:
(a) Derive Eq.5.8.1.
(b) Derive an expression for the voltage drop in the poly-depletion region, i.e. the
band bending in the poly-Si gate, s. Assume that the electric field inside the
oxide ,ox, is known.
(c) Continue from (b) and express poly in terms of Vg, not ox. Assume surface in
version, i.e. Vg  Vt. Other usual MOS parameters such as Vfb, Tox, B may also
appear. Hint: Vg = Vfb + Vox + 2B + poly.
(d) Using the result of (c), find an expression for Wdpoly in terms of Vg, not ox.
For part (e), (f), and (g), assume Tox = 2nm, Na = 1017cm-3, Nd = 61019cm-3 (for
N+-poly-gate), and Vg = 1.5V.
(e) Evaluate poly and Wdpoly.
(f) Calculate Vt using Eq. 5.4.3. (The poly-depletion effect maybe ignored in Vt
calculation because ox is very low at Vg=Vt.) Then, using poly from part (e) in
Eq. 5.8.3, find Qinv.
(g) Calculate Qinv = Coxe(Vg-Vt) with Coxe given by Eq. 5.8.2.
Discussion:
Eq. 5.8.2 is correct for a small signal capacitor. In this case,
C V g   dQV g  / dV g  QV g    C V g dV g
where C and Q are functions of Vg. Hence, solving the integral above will not yield
the same result you obtained for part (f) since C varies with Vg due to the polydepletion effect. The answer for part (f) is the correct value for Qinv.
```